# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2021

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_JW-20
_database_code_depnum_ccdc_archive 'CCDC 2062084'
loop_
_audit_author_name
_audit_author_address
'Yan Xu'
;Nanjing Tech University
China
;
_audit_update_record             
;
2021-05-13 deposited with the CCDC.	2021-05-24 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2018/3
_shelx_SHELXL_version_number     2018/3
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C30 H71.33 Co5.33 Mo12 N12 O70 P8'
_chemical_formula_weight         3433.65

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_H-M_alt        'C 2/c'
_space_group_name_Hall           '-C 2yc'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   30.375(4)
_cell_length_b                   14.5133(14)
_cell_length_c                   24.714(3)
_cell_angle_alpha                90
_cell_angle_beta                 123.811(2)
_cell_angle_gamma                90
_cell_volume                     9052.5(17)
_cell_formula_units_Z            4
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    7746
_cell_measurement_theta_min      4.369
_cell_measurement_theta_max      53.651

_exptl_crystal_description       blocky
_exptl_crystal_colour            black
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    2.519
_exptl_crystal_F_000             6653
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.150
_exptl_crystal_size_mid          0.120
_exptl_crystal_size_min          0.100
_exptl_absorpt_coefficient_mu    2.809
_shelx_estimated_absorpt_T_min   0.678
_shelx_estimated_absorpt_T_max   0.766
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.683
_exptl_absorpt_correction_T_max  0.771
_exptl_absorpt_process_details   '(SADABS; Sheldrick, 2003)'
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker Apex2 CCD'
_diffrn_measurement_method       'ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            32307
_diffrn_reflns_av_unetI/netI     0.0462
_diffrn_reflns_av_R_equivalents  0.0620
_diffrn_reflns_limit_h_min       -36
_diffrn_reflns_limit_h_max       36
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_l_min       -29
_diffrn_reflns_limit_l_max       27
_diffrn_reflns_theta_min         1.614
_diffrn_reflns_theta_max         25.099
_diffrn_reflns_theta_full        25.099
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measured_fraction_theta_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_point_group_measured_fraction_full 0.997
_reflns_number_total             8040
_reflns_number_gt                6542
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       'APEX2 (Bruker, 2005)'
_computing_cell_refinement       'SAINT (Bruker, 2005)'
_computing_data_reduction        SAINT
_computing_structure_solution    'SHELXT 2018/3 (Sheldrick, 2018)'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_molecular_graphics    SHELXTL
_computing_publication_material  SHELXTL
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.1008P)²+130.8909P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   mixed
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         8040
_refine_ls_number_parameters     648
_refine_ls_number_restraints     311
_refine_ls_R_factor_all          0.0714
_refine_ls_R_factor_gt           0.0575
_refine_ls_wR_factor_ref         0.1742
_refine_ls_wR_factor_gt          0.1630
_refine_ls_goodness_of_fit_ref   1.094
_refine_ls_restrained_S_all      1.395
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.13308(3) 0.61300(5) 0.47609(3) 0.0209(2) Uani 1 1 d . . . . .
Mo2 Mo 0.19140(3) 0.96110(5) 0.39245(4) 0.0238(2) Uani 1 1 d . . . . .
Mo3 Mo 0.14038(3) 0.76884(5) 0.53134(4) 0.0235(2) Uani 1 1 d . . . . .
Mo4 Mo 0.17718(3) 0.96990(5) 0.48648(4) 0.0253(2) Uani 1 1 d . . . . .
Mo5 Mo 0.17810(3) 0.75378(6) 0.31406(3) 0.0237(2) Uani 1 1 d . . . . .
Mo6 Mo 0.15261(3) 0.60666(6) 0.34974(4) 0.0309(2) Uani 1 1 d . . . . .
Co1 Co 0.250000 0.750000 0.500000 0.0190(3) Uani 1 2 d S . P . .
Co2 Co 0.000000 0.92498(13) 0.250000 0.0369(5) Uani 1 2 d S T P B .
Co3 Co 0.03440(7) 0.76330(14) 0.21079(10) 0.0353(5) Uani 0.6667 1 d . U P B .
Co4 Co -0.03982(5) 1.02610(9) 0.40815(6) 0.0280(3) Uani 1 1 d . . . . .
P1A P 0.07244(19) 0.4625(3) 0.3530(2) 0.0295(11) Uani 0.5 1 d . U P A 1
O1 O 0.1111(6) 0.3794(10) 0.3912(8) 0.051(4) Uani 0.5 1 d . U P A 1
P1B P 0.04120(19) 0.5244(4) 0.3352(2) 0.0353(12) Uani 0.5 1 d D U P A 2
O2 O -0.0076(5) 0.5835(12) 0.3024(8) 0.049(4) Uani 0.5 1 d D U P A 2
P2 P 0.10044(8) 0.79828(16) 0.37188(10) 0.0214(5) Uani 1 1 d . . . . .
P3 P 0.07183(9) 0.96368(17) 0.49318(12) 0.0284(5) Uani 1 1 d . . . . .
P4 P 0.10772(9) 0.93530(18) 0.23423(11) 0.0306(6) Uani 1 1 d . . . . .
O3 O 0.1904(2) 0.7064(4) 0.5162(3) 0.0220(12) Uani 1 1 d . U . . .
O4 O 0.1740(2) 0.5520(4) 0.4393(3) 0.0242(13) Uani 1 1 d . . . . .
O5 O 0.1924(2) 0.8811(4) 0.5616(3) 0.0264(13) Uani 1 1 d . . . . .
O6 O 0.2101(2) 0.6962(4) 0.4008(3) 0.0212(12) Uani 1 1 d . . . . .
O7 O 0.0713(2) 0.5305(5) 0.4058(3) 0.0339(16) Uani 1 1 d . . . . .
O8 O 0.2213(2) 0.8861(4) 0.4729(3) 0.0208(12) Uani 1 1 d . . . . .
O9 O 0.1373(2) 0.8368(4) 0.3525(3) 0.0238(13) Uani 1 1 d . . . . .
O10 O 0.1378(2) 1.0204(4) 0.3991(3) 0.0310(15) Uani 1 1 d . . . . .
O11 O 0.0889(3) 0.8669(5) 0.5231(3) 0.0339(15) Uani 1 1 d . . . . .
O12 O 0.1114(2) 0.6934(4) 0.3850(3) 0.0242(13) Uani 1 1 d . . . . .
O13 O 0.2272(2) 0.8660(4) 0.3635(3) 0.0240(13) Uani 1 1 d . . . . .
O14 O 0.0800(2) 0.6909(4) 0.4726(3) 0.0288(14) Uani 1 1 d . . . . .
O15 O 0.1122(3) 0.6846(6) 0.2728(3) 0.046(2) Uani 1 1 d . . . . .
O17 O 0.1432(3) 0.9937(5) 0.2956(3) 0.0410(18) Uani 1 1 d . . . . .
O18 O 0.1519(3) 0.5405(4) 0.5380(3) 0.0321(15) Uani 1 1 d . . . . .
O19 O 0.0429(2) 0.8118(4) 0.3168(3) 0.0251(13) Uani 1 1 d . . . . .
O20 O 0.2374(2) 1.0427(4) 0.4149(3) 0.0311(15) Uani 1 1 d . . . . .
O21 O -0.0590(3) 0.9779(4) 0.4657(4) 0.0374(16) Uani 1 1 d . . . . .
O23 O 0.1369(2) 0.8456(5) 0.2392(3) 0.0361(16) Uani 1 1 d . . . . .
O24 O 0.0827(3) 0.5330(6) 0.3127(4) 0.063(3) Uani 1 1 d . . . . .
O25 O 0.1169(2) 0.8453(4) 0.4360(3) 0.0225(13) Uani 1 1 d . . . . .
O26 O 0.2130(3) 0.7058(5) 0.2869(3) 0.0380(16) Uani 1 1 d . . . . .
O27 O 0.0219(3) 0.9573(5) 0.4234(3) 0.0374(16) Uani 1 1 d . . . . .
O28 O 0.1161(2) 1.0127(4) 0.4923(3) 0.0316(15) Uani 1 1 d . . . . .
O29 O 0.2202(3) 1.0532(5) 0.5324(3) 0.0358(16) Uani 1 1 d . . . . .
O30 O 0.0550(2) 0.9092(5) 0.2243(3) 0.0364(16) Uani 1 1 d . . . . .
O31 O 0.0193(3) 0.4246(6) 0.3100(4) 0.052(2) Uani 1 1 d . . . . .
O32 O 0.1606(3) 0.7315(5) 0.6062(3) 0.0357(16) Uani 1 1 d . . . . .
O33 O 0.1822(4) 0.5278(5) 0.3306(4) 0.057(2) Uani 1 1 d . . . . .
O34 O -0.1003(3) 0.9904(6) 0.3230(3) 0.060(3) Uani 1 1 d . . . . .
N1 N -0.0311(3) 1.1601(5) 0.4018(3) 0.045(2) Uani 1 1 d D U . . .
N2 N -0.0061(5) 1.3110(5) 0.4339(4) 0.084(4) Uani 1 1 d D U . . .
N3 N -0.1790(4) 1.1770(8) 0.2134(5) 0.108(4) Uani 1 1 d D U . . .
H3A H -0.166175 1.122923 0.216746 0.130 Uiso 1 1 calc R U . . .
N4 N -0.2156(4) 1.2995(5) 0.2275(4) 0.114(4) Uani 1 1 d D U . . .
N5 N -0.1429(4) 1.6799(6) 0.3839(5) 0.108(4) Uani 1 1 d D U . . .
N6 N -0.1635(6) 1.7516(7) 0.4474(6) 0.134(5) Uani 1 1 d D U . . .
H6 H -0.171193 1.762651 0.475471 0.161 Uiso 1 1 calc R U . . .
C1 C -0.0064(6) 1.2222(5) 0.4513(5) 0.088(4) Uani 1 1 d D U . . .
H1 H 0.009327 1.204950 0.494511 0.106 Uiso 1 1 calc R U . . .
C2 C -0.0487(7) 1.2141(6) 0.3485(4) 0.114(6) Uani 1 1 d D U . . .
H2 H -0.064815 1.193365 0.305937 0.136 Uiso 1 1 calc R U . . .
C3 C -0.0388(6) 1.3037(7) 0.3680(4) 0.099(5) Uani 1 1 d D U . . .
H3 H -0.052771 1.353698 0.339791 0.119 Uiso 1 1 calc R U . . .
C4 C 0.0225(4) 1.3910(7) 0.4764(7) 0.108(6) Uani 1 1 d D U . . .
H4A H 0.042775 1.420923 0.461991 0.130 Uiso 1 1 calc R U . . .
H4B H 0.047062 1.369838 0.520727 0.130 Uiso 1 1 calc R U . . .
C5 C -0.0160(5) 1.4605(9) 0.4751(8) 0.101(6) Uani 1 1 d D U . . .
H5A H -0.038258 1.429863 0.486372 0.121 Uiso 1 1 calc R U . . .
H5B H -0.038675 1.485965 0.431689 0.121 Uiso 1 1 calc R U . . .
C6 C -0.2060(5) 1.3230(9) 0.1809(5) 0.151(9) Uani 1 1 d D U . . .
H6A H -0.212935 1.379352 0.159736 0.182 Uiso 1 1 calc R U . . .
C7 C -0.1839(6) 1.2462(7) 0.1721(6) 0.104(5) Uani 1 1 d D U . . .
H7 H -0.173792 1.241743 0.142864 0.124 Uiso 1 1 calc R U . . .
C8 C -0.1986(5) 1.2105(6) 0.2482(5) 0.084(3) Uani 1 1 d D U . . .
H8 H -0.200128 1.178826 0.279911 0.101 Uiso 1 1 calc DR U . . .
C9 C -0.2283(4) 1.3855(7) 0.2504(7) 0.140(5) Uani 1 1 d D U . . .
H9A H -0.226273 1.359184 0.287367 0.168 Uiso 1 1 d R U . . .
H9B H -0.262913 1.411784 0.222427 0.168 Uiso 1 1 d R U . . .
C10 C -0.1783(5) 1.4394(8) 0.2995(9) 0.153(5) Uani 1 1 d D U . . .
H10A H -0.160371 1.455754 0.278873 0.184 Uiso 1 1 d DR U . . .
H10B H -0.154231 1.405846 0.338743 0.184 Uiso 1 1 d R U . . .
C11 C -0.1907(5) 1.5355(8) 0.3130(10) 0.148(5) Uani 1 1 d D U . . .
H11A H -0.204037 1.520756 0.339235 0.178 Uiso 1 1 d R U . . .
H11B H -0.218137 1.565045 0.273645 0.178 Uiso 1 1 d DR U . . .
C12 C -0.1394(5) 1.5909(8) 0.3533(8) 0.125(5) Uani 1 1 d D U . . .
H12A H -0.112756 1.551618 0.387943 0.150 Uiso 1 1 calc R U . . .
H12B H -0.127144 1.606302 0.325618 0.150 Uiso 1 1 calc R U . . .
C13 C -0.1273(5) 1.7700(6) 0.3866(6) 0.117(5) Uani 1 1 d D U . . .
H13 H -0.109466 1.795738 0.369556 0.141 Uiso 1 1 calc R U . . .
C14 C -0.1449(5) 1.8118(10) 0.4213(5) 0.131(5) Uani 1 1 d D U . . .
H14 H -0.144336 1.875360 0.426701 0.157 Uiso 1 1 calc R U . . .
C15 C -0.1668(5) 1.6693(8) 0.4174(5) 0.121(5) Uani 1 1 d D U . . .
H15 H -0.182459 1.615582 0.419504 0.145 Uiso 1 1 calc R U . . .
O1W O -0.1880(6) 1.0216(10) 0.3350(7) 0.144(6) Uani 1 1 d D U . . .
H1WA H -0.194834 1.065809 0.352338 0.215 Uiso 1 1 d DR U . . .
H1WB H -0.169514 1.042469 0.321148 0.215 Uiso 1 1 d DR U . . .
O2W O 0.000000 1.2082(17) 0.250000 0.252(17) Uani 1 2 d DS TU P . .
H2WA H -0.018810 1.178870 0.210930 0.378 Uiso 1 1 d DR U . . .
O4W O -0.0341(2) 1.0211(5) 0.1758(3) 0.0383(17) Uani 1 1 d D . . . .
O5W O 0.0161(3) 0.7764(6) 0.1096(5) 0.066(3) Uani 1 1 d . U . . .
O3W O 0.0113(6) 0.6317(12) 0.1886(7) 0.044(4) Uani 0.5 1 d . U P B 1


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O18 1.674(6) . ?
Mo1 O14 1.931(6) . ?
Mo1 O3 1.982(6) . ?
Mo1 O7 2.084(6) . ?
Mo1 O4 2.102(6) . ?
Mo1 O12 2.283(6) . ?
Mo1 Mo3 2.5868(11) . ?
Mo2 O20 1.673(6) . ?
Mo2 O10 1.928(6) . ?
Mo2 O8 1.987(5) . ?
Mo2 O17 2.048(6) . ?
Mo2 O13 2.112(6) . ?
Mo2 O9 2.264(6) . ?
Mo2 Mo4 2.5924(12) . ?
Mo3 O32 1.682(6) . ?
Mo3 O14 1.946(6) . ?
Mo3 O3 1.975(6) . ?
Mo3 O11 2.040(6) . ?
Mo3 O5 2.097(6) . ?
Mo3 O25 2.328(5) . ?
Mo4 O29 1.675(7) . ?
Mo4 O10 1.937(6) . ?
Mo4 O8 1.973(6) . ?
Mo4 O28 2.037(6) . ?
Mo4 O5 2.089(6) . ?
Mo4 O25 2.375(6) . ?
Mo5 O26 1.687(7) . ?
Mo5 O15 1.945(6) . ?
Mo5 O6 1.981(5) . ?
Mo5 O23 2.046(6) . ?
Mo5 O13 2.084(6) . ?
Mo5 O9 2.281(6) . ?
Mo5 Mo6 2.5877(11) . ?
Mo6 O33 1.677(8) . ?
Mo6 O15 1.951(7) . ?
Mo6 O6 1.969(6) . ?
Mo6 O24 2.081(7) . ?
Mo6 O4 2.085(6) . ?
Mo6 O12 2.264(6) . ?
Co1 O8 2.112(6) 7_566 ?
Co1 O8 2.112(6) . ?
Co1 O3 2.155(6) . ?
Co1 O3 2.155(6) 7_566 ?
Co1 O6 2.186(5) . ?
Co1 O6 2.186(5) 7_566 ?
Co2 O4W 2.066(7) . ?
Co2 O4W 2.066(7) 2 ?
Co2 O30 2.105(7) . ?
Co2 O30 2.105(7) 2 ?
Co2 O19 2.174(6) 2 ?
Co2 O19 2.174(6) . ?
Co2 Co3 2.943(3) 2 ?
Co2 Co3 2.943(3) . ?
Co3 O3W 2.004(17) . ?
Co3 O19 2.167(6) 2 ?
Co3 O30 2.181(7) . ?
Co3 O5W 2.247(11) . ?
Co3 O15 2.283(8) . ?
Co4 O21 1.941(7) . ?
Co4 O34 1.942(7) . ?
Co4 O27 1.966(6) . ?
Co4 N1 1.981(8) . ?
P1A O31 1.459(9) . ?
P1A O24 1.575(9) . ?
P1A O1 1.578(15) . ?
P1A O7 1.652(9) . ?
P1B O7 1.454(8) . ?
P1B O2 1.501(9) . ?
P1B O31 1.571(9) . ?
P1B O24 1.641(10) . ?
P2 O19 1.516(6) . ?
P2 O25 1.531(6) . ?
P2 O9 1.546(6) . ?
P2 O12 1.553(6) . ?
P3 O28 1.532(7) . ?
P3 O21 1.533(7) 5_576 ?
P3 O11 1.537(7) . ?
P3 O27 1.540(7) . ?
P4 O30 1.526(7) . ?
P4 O34 1.528(7) 2 ?
P4 O17 1.537(7) . ?
P4 O23 1.541(8) . ?
N1 C1 1.3600(5) . ?
N1 C2 1.3600(5) . ?
N2 C3 1.3599(5) . ?
N2 C1 1.3600(5) . ?
N2 C4 1.4800(5) . ?
N3 C8 1.3800(5) . ?
N3 C7 1.3800(5) . ?
N3 H3A 0.8600 . ?
N4 C8 1.3800(5) . ?
N4 C6 1.3800(5) . ?
N4 C9 1.5050(4) . ?
N5 C13 1.3800(5) . ?
N5 C15 1.3800(5) . ?
N5 C12 1.5300(5) . ?
N6 C15 1.3800(5) . ?
N6 C14 1.3800(5) . ?
N6 H6 0.8600 . ?
C1 H1 0.9300 . ?
C2 C3 1.3600(5) . ?
C2 H2 0.9300 . ?
C3 H3 0.9300 . ?
C4 C5 1.5300(5) . ?
C4 H4A 0.9700 . ?
C4 H4B 0.9700 . ?
C5 C5 1.56(3) 5_586 ?
C5 H5A 0.9700 . ?
C5 H5B 0.9700 . ?
C6 C7 1.3800(5) . ?
C6 H6A 0.9300 . ?
C7 H7 0.9300 . ?
C8 H8 0.9300 . ?
C9 C10 1.5300(5) . ?
C9 H9A 0.9600 . ?
C9 H9B 0.9600 . ?
C10 C11 1.5299(5) . ?
C10 H10A 0.9599 . ?
C10 H10B 0.9601 . ?
C11 C12 1.5300(6) . ?
C11 H11A 0.9600 . ?
C11 H11B 0.9600 . ?
C12 H12A 0.9700 . ?
C12 H12B 0.9700 . ?
C13 C14 1.3800(5) . ?
C13 H13 0.9300 . ?
C14 H14 0.9300 . ?
C15 H15 0.9300 . ?
O1W H1WA 0.8596 . ?
O1W H1WB 0.8590 . ?
O2W H2WA 0.9089 . ?
O2W H2WA 0.9088 2 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O18 Mo1 O14 105.1(3) . . ?
O18 Mo1 O3 102.4(3) . . ?
O14 Mo1 O3 95.8(3) . . ?
O18 Mo1 O7 95.2(3) . . ?
O14 Mo1 O7 87.5(3) . . ?
O3 Mo1 O7 160.4(2) . . ?
O18 Mo1 O4 98.5(3) . . ?
O14 Mo1 O4 155.2(2) . . ?
O3 Mo1 O4 86.4(2) . . ?
O7 Mo1 O4 82.7(3) . . ?
O18 Mo1 O12 170.8(3) . . ?
O14 Mo1 O12 83.1(2) . . ?
O3 Mo1 O12 80.5(2) . . ?
O7 Mo1 O12 80.8(2) . . ?
O4 Mo1 O12 72.8(2) . . ?
O18 Mo1 Mo3 100.5(2) . . ?
O14 Mo1 Mo3 48.40(19) . . ?
O3 Mo1 Mo3 49.06(17) . . ?
O7 Mo1 Mo3 135.7(2) . . ?
O4 Mo1 Mo3 134.35(17) . . ?
O12 Mo1 Mo3 88.10(16) . . ?
O20 Mo2 O10 104.2(3) . . ?
O20 Mo2 O8 102.9(3) . . ?
O10 Mo2 O8 95.6(3) . . ?
O20 Mo2 O17 98.4(3) . . ?
O10 Mo2 O17 84.8(3) . . ?
O8 Mo2 O17 158.0(2) . . ?
O20 Mo2 O13 94.7(3) . . ?
O10 Mo2 O13 159.8(2) . . ?
O8 Mo2 O13 86.9(2) . . ?
O17 Mo2 O13 85.6(3) . . ?
O20 Mo2 O9 168.0(3) . . ?
O10 Mo2 O9 87.1(2) . . ?
O8 Mo2 O9 79.4(2) . . ?
O17 Mo2 O9 78.6(2) . . ?
O13 Mo2 O9 73.6(2) . . ?
O20 Mo2 Mo4 101.1(2) . . ?
O10 Mo2 Mo4 48.04(19) . . ?
O8 Mo2 Mo4 48.87(17) . . ?
O17 Mo2 Mo4 132.0(2) . . ?
O13 Mo2 Mo4 135.17(16) . . ?
O9 Mo2 Mo4 89.27(15) . . ?
O32 Mo3 O14 104.4(3) . . ?
O32 Mo3 O3 102.3(3) . . ?
O14 Mo3 O3 95.5(2) . . ?
O32 Mo3 O11 97.1(3) . . ?
O14 Mo3 O11 88.8(3) . . ?
O3 Mo3 O11 158.3(3) . . ?
O32 Mo3 O5 96.8(3) . . ?
O14 Mo3 O5 158.1(2) . . ?
O3 Mo3 O5 85.2(2) . . ?
O11 Mo3 O5 83.0(3) . . ?
O32 Mo3 O25 170.2(3) . . ?
O14 Mo3 O25 83.7(2) . . ?
O3 Mo3 O25 82.0(2) . . ?
O11 Mo3 O25 77.3(2) . . ?
O5 Mo3 O25 74.7(2) . . ?
O32 Mo3 Mo1 99.8(2) . . ?
O14 Mo3 Mo1 47.89(18) . . ?
O3 Mo3 Mo1 49.30(17) . . ?
O11 Mo3 Mo1 136.2(2) . . ?
O5 Mo3 Mo1 133.91(17) . . ?
O25 Mo3 Mo1 89.68(15) . . ?
O29 Mo4 O10 104.3(3) . . ?
O29 Mo4 O8 102.3(3) . . ?
O10 Mo4 O8 95.7(3) . . ?
O29 Mo4 O28 97.4(3) . . ?
O10 Mo4 O28 86.6(3) . . ?
O8 Mo4 O28 158.8(2) . . ?
O29 Mo4 O5 98.0(3) . . ?
O10 Mo4 O5 156.6(2) . . ?
O8 Mo4 O5 86.3(2) . . ?
O28 Mo4 O5 83.4(2) . . ?
O29 Mo4 O25 171.2(3) . . ?
O10 Mo4 O25 83.4(2) . . ?
O8 Mo4 O25 80.8(2) . . ?
O28 Mo4 O25 78.6(2) . . ?
O5 Mo4 O25 73.8(2) . . ?
O29 Mo4 Mo2 100.8(2) . . ?
O10 Mo4 Mo2 47.72(19) . . ?
O8 Mo4 Mo2 49.35(15) . . ?
O28 Mo4 Mo2 133.72(18) . . ?
O5 Mo4 Mo2 134.49(17) . . ?
O25 Mo4 Mo2 87.48(14) . . ?
O26 Mo5 O15 105.6(3) . . ?
O26 Mo5 O6 102.6(3) . . ?
O15 Mo5 O6 95.3(3) . . ?
O26 Mo5 O23 96.5(3) . . ?
O15 Mo5 O23 85.9(3) . . ?
O6 Mo5 O23 159.8(3) . . ?
O26 Mo5 O13 98.8(3) . . ?
O15 Mo5 O13 154.5(3) . . ?
O6 Mo5 O13 86.3(2) . . ?
O23 Mo5 O13 84.2(3) . . ?
O26 Mo5 O9 172.1(3) . . ?
O15 Mo5 O9 81.5(3) . . ?
O6 Mo5 O9 79.9(2) . . ?
O23 Mo5 O9 80.3(2) . . ?
O13 Mo5 O9 73.7(2) . . ?
O26 Mo5 Mo6 99.7(2) . . ?
O15 Mo5 Mo6 48.5(2) . . ?
O6 Mo5 Mo6 48.87(16) . . ?
O23 Mo5 Mo6 134.19(19) . . ?
O13 Mo5 Mo6 134.19(16) . . ?
O9 Mo5 Mo6 87.64(15) . . ?
O33 Mo6 O15 105.4(4) . . ?
O33 Mo6 O6 102.0(4) . . ?
O15 Mo6 O6 95.4(3) . . ?
O33 Mo6 O24 95.8(4) . . ?
O15 Mo6 O24 86.2(3) . . ?
O6 Mo6 O24 160.9(3) . . ?
O33 Mo6 O4 98.0(3) . . ?
O15 Mo6 O4 155.7(3) . . ?
O6 Mo6 O4 85.9(2) . . ?
O24 Mo6 O4 84.9(3) . . ?
O33 Mo6 O12 170.2(3) . . ?
O15 Mo6 O12 82.6(3) . . ?
O6 Mo6 O12 82.5(2) . . ?
O24 Mo6 O12 78.9(3) . . ?
O4 Mo6 O12 73.5(2) . . ?
O33 Mo6 Mo5 99.1(3) . . ?
O15 Mo6 Mo5 48.27(19) . . ?
O6 Mo6 Mo5 49.27(16) . . ?
O24 Mo6 Mo5 134.4(2) . . ?
O4 Mo6 Mo5 134.40(17) . . ?
O12 Mo6 Mo5 90.40(15) . . ?
O8 Co1 O8 180.0 7_566 . ?
O8 Co1 O3 84.7(2) 7_566 . ?
O8 Co1 O3 95.3(2) . . ?
O8 Co1 O3 95.3(2) 7_566 7_566 ?
O8 Co1 O3 84.7(2) . 7_566 ?
O3 Co1 O3 180.0 . 7_566 ?
O8 Co1 O6 84.0(2) 7_566 . ?
O8 Co1 O6 96.0(2) . . ?
O3 Co1 O6 96.0(2) . . ?
O3 Co1 O6 84.0(2) 7_566 . ?
O8 Co1 O6 96.0(2) 7_566 7_566 ?
O8 Co1 O6 84.0(2) . 7_566 ?
O3 Co1 O6 84.0(2) . 7_566 ?
O3 Co1 O6 96.0(2) 7_566 7_566 ?
O6 Co1 O6 180.0 . 7_566 ?
O4W Co2 O4W 95.1(4) . 2 ?
O4W Co2 O30 84.0(3) . . ?
O4W Co2 O30 104.5(3) 2 . ?
O4W Co2 O30 104.5(3) . 2 ?
O4W Co2 O30 84.0(3) 2 2 ?
O30 Co2 O30 167.5(4) . 2 ?
O4W Co2 O19 92.5(2) . 2 ?
O4W Co2 O19 167.6(3) 2 2 ?
O30 Co2 O19 86.0(2) . 2 ?
O30 Co2 O19 84.6(2) 2 2 ?
O4W Co2 O19 167.6(3) . . ?
O4W Co2 O19 92.5(2) 2 . ?
O30 Co2 O19 84.6(2) . . ?
O30 Co2 O19 86.0(2) 2 . ?
O19 Co2 O19 81.8(3) 2 . ?
O4W Co2 Co3 137.36(18) . 2 ?
O4W Co2 Co3 109.9(2) 2 2 ?
O30 Co2 Co3 120.0(2) . 2 ?
O30 Co2 Co3 47.7(2) 2 2 ?
O19 Co2 Co3 58.31(17) 2 2 ?
O19 Co2 Co3 47.20(16) . 2 ?
O4W Co2 Co3 109.9(2) . . ?
O4W Co2 Co3 137.36(18) 2 . ?
O30 Co2 Co3 47.7(2) . . ?
O30 Co2 Co3 120.0(2) 2 . ?
O19 Co2 Co3 47.20(15) 2 . ?
O19 Co2 Co3 58.31(17) . . ?
Co3 Co2 Co3 74.28(9) 2 . ?
O3W Co3 O19 94.1(5) . 2 ?
O3W Co3 O30 174.1(5) . . ?
O19 Co3 O30 84.3(2) 2 . ?
O3W Co3 O5W 86.8(5) . . ?
O19 Co3 O5W 94.0(3) 2 . ?
O30 Co3 O5W 87.7(3) . . ?
O3W Co3 O15 77.3(5) . . ?
O19 Co3 O15 155.5(2) 2 . ?
O30 Co3 O15 106.3(3) . . ?
O5W Co3 O15 108.1(3) . . ?
O3W Co3 Co2 135.7(5) . . ?
O19 Co3 Co2 47.42(16) 2 . ?
O30 Co3 Co2 45.56(19) . . ?
O5W Co3 Co2 112.7(2) . . ?
O15 Co3 Co2 127.1(2) . . ?
O21 Co4 O34 102.1(4) . . ?
O21 Co4 O27 108.6(3) . . ?
O34 Co4 O27 107.4(3) . . ?
O21 Co4 N1 121.3(3) . . ?
O34 Co4 N1 105.3(4) . . ?
O27 Co4 N1 111.0(3) . . ?
O31 P1A O24 108.2(5) . . ?
O31 P1A O1 107.5(7) . . ?
O24 P1A O1 122.2(8) . . ?
O31 P1A O7 107.4(5) . . ?
O24 P1A O7 102.2(5) . . ?
O1 P1A O7 108.6(7) . . ?
O7 P1B O2 112.7(8) . . ?
O7 P1B O31 112.2(5) . . ?
O2 P1B O31 103.8(8) . . ?
O7 P1B O24 108.3(5) . . ?
O2 P1B O24 119.2(9) . . ?
O31 P1B O24 99.9(5) . . ?
O19 P2 O25 114.9(3) . . ?
O19 P2 O9 110.2(3) . . ?
O25 P2 O9 106.5(3) . . ?
O19 P2 O12 108.6(3) . . ?
O25 P2 O12 108.2(3) . . ?
O9 P2 O12 108.2(3) . . ?
O28 P3 O21 107.6(4) . 5_576 ?
O28 P3 O11 111.6(4) . . ?
O21 P3 O11 109.1(4) 5_576 . ?
O28 P3 O27 109.7(4) . . ?
O21 P3 O27 108.7(4) 5_576 . ?
O11 P3 O27 110.0(4) . . ?
O30 P4 O34 112.3(4) . 2 ?
O30 P4 O17 113.1(4) . . ?
O34 P4 O17 106.6(4) 2 . ?
O30 P4 O23 108.0(4) . . ?
O34 P4 O23 107.4(5) 2 . ?
O17 P4 O23 109.3(4) . . ?
Mo3 O3 Mo1 81.6(2) . . ?
Mo3 O3 Co1 135.6(3) . . ?
Mo1 O3 Co1 134.7(3) . . ?
Mo6 O4 Mo1 112.9(3) . . ?
Mo4 O5 Mo3 114.4(3) . . ?
Mo6 O6 Mo5 81.9(2) . . ?
Mo6 O6 Co1 134.1(3) . . ?
Mo5 O6 Co1 134.0(3) . . ?
P1B O7 Mo1 135.1(4) . . ?
P1A O7 Mo1 126.6(4) . . ?
Mo4 O8 Mo2 81.8(2) . . ?
Mo4 O8 Co1 136.2(3) . . ?
Mo2 O8 Co1 135.1(3) . . ?
P2 O9 Mo2 128.9(4) . . ?
P2 O9 Mo5 126.3(4) . . ?
Mo2 O9 Mo5 99.9(2) . . ?
Mo2 O10 Mo4 84.2(2) . . ?
P3 O11 Mo3 136.0(4) . . ?
P2 O12 Mo6 124.4(3) . . ?
P2 O12 Mo1 128.1(3) . . ?
Mo6 O12 Mo1 100.2(2) . . ?
Mo5 O13 Mo2 112.0(3) . . ?
Mo1 O14 Mo3 83.7(2) . . ?
Mo5 O15 Mo6 83.3(3) . . ?
Mo5 O15 Co3 118.2(4) . . ?
Mo6 O15 Co3 143.0(4) . . ?
P4 O17 Mo2 132.7(4) . . ?
P2 O19 Co3 138.3(4) . 2 ?
P2 O19 Co2 133.2(4) . . ?
Co3 O19 Co2 85.4(2) 2 . ?
P3 O21 Co4 125.3(4) 5_576 . ?
P4 O23 Mo5 131.1(4) . . ?
P1A O24 Mo6 124.6(5) . . ?
P1B O24 Mo6 132.7(5) . . ?
P2 O25 Mo3 125.1(3) . . ?
P2 O25 Mo4 126.5(3) . . ?
Mo3 O25 Mo4 96.8(2) . . ?
P3 O27 Co4 115.1(4) . . ?
P3 O28 Mo4 134.5(4) . . ?
P4 O30 Co2 149.6(4) . . ?
P4 O30 Co3 116.8(4) . . ?
Co2 O30 Co3 86.7(3) . . ?
P4 O34 Co4 134.9(5) 2 . ?
C1 N1 C2 102.2(8) . . ?
C1 N1 Co4 127.6(6) . . ?
C2 N1 Co4 130.2(7) . . ?
C3 N2 C1 100.0(8) . . ?
C3 N2 C4 131.4(10) . . ?
C1 N2 C4 128.6(9) . . ?
C8 N3 C7 107.5(11) . . ?
C8 N3 H3A 126.3 . . ?
C7 N3 H3A 126.3 . . ?
C8 N4 C6 109.4(10) . . ?
C8 N4 C9 139.2(10) . . ?
C6 N4 C9 109.0(10) . . ?
C13 N5 C15 110.9(10) . . ?
C13 N5 C12 135.0(11) . . ?
C15 N5 C12 114.0(10) . . ?
C15 N6 C14 102.9(13) . . ?
C15 N6 H6 128.6 . . ?
C14 N6 H6 128.6 . . ?
N2 C1 N1 116.2(8) . . ?
N2 C1 H1 121.9 . . ?
N1 C1 H1 121.9 . . ?
C3 C2 N1 108.5(9) . . ?
C3 C2 H2 125.8 . . ?
N1 C2 H2 125.8 . . ?
N2 C3 C2 111.7(9) . . ?
N2 C3 H3 124.2 . . ?
C2 C3 H3 124.2 . . ?
N2 C4 C5 111.2(10) . . ?
N2 C4 H4A 109.4 . . ?
C5 C4 H4A 109.4 . . ?
N2 C4 H4B 109.4 . . ?
C5 C4 H4B 109.4 . . ?
H4A C4 H4B 108.0 . . ?
C4 C5 C5 109.5(11) . 5_586 ?
C4 C5 H5A 109.8 . . ?
C5 C5 H5A 109.8 5_586 . ?
C4 C5 H5B 109.8 . . ?
C5 C5 H5B 109.8 5_586 . ?
H5A C5 H5B 108.2 . . ?
C7 C6 N4 106.3(11) . . ?
C7 C6 H6A 126.8 . . ?
N4 C6 H6A 126.8 . . ?
N3 C7 C6 109.3(12) . . ?
N3 C7 H7 125.3 . . ?
C6 C7 H7 125.3 . . ?
N3 C8 N4 107.5(9) . . ?
N3 C8 H8 126.3 . . ?
N4 C8 H8 126.3 . . ?
N4 C9 C10 112.0(8) . . ?
N4 C9 H9A 97.7 . . ?
C10 C9 H9A 86.5 . . ?
N4 C9 H9B 117.8 . . ?
C10 C9 H9B 125.0 . . ?
H9A C9 H9B 107.9 . . ?
C11 C10 C9 112.5(8) . . ?
C11 C10 H10A 99.9 . . ?
C9 C10 H10A 108.1 . . ?
C11 C10 H10B 112.6 . . ?
C9 C10 H10B 113.8 . . ?
H10A C10 H10B 108.9 . . ?
C10 C11 C12 109.6(8) . . ?
C10 C11 H11A 101.1 . . ?
C12 C11 H11A 109.7 . . ?
C10 C11 H11B 111.5 . . ?
C12 C11 H11B 114.9 . . ?
H11A C11 H11B 109.3 . . ?
N5 C12 C11 116.0(9) . . ?
N5 C12 H12A 108.3 . . ?
C11 C12 H12A 108.3 . . ?
N5 C12 H12B 108.3 . . ?
C11 C12 H12B 108.3 . . ?
H12A C12 H12B 107.4 . . ?
N5 C13 C14 101.9(11) . . ?
N5 C13 H13 129.1 . . ?
C14 C13 H13 129.1 . . ?
C13 C14 N6 114.4(13) . . ?
C13 C14 H14 122.8 . . ?
N6 C14 H14 122.8 . . ?
N6 C15 N5 108.8(11) . . ?
N6 C15 H15 125.6 . . ?
N5 C15 H15 125.6 . . ?
H1WA O1W H1WB 109.1 . . ?
H2WA O2W H2WA 124.1 . 2 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O2 P1B O7 Mo1 -90.8(10) . . . . ?
O31 P1B O7 Mo1 152.5(6) . . . . ?
O24 P1B O7 Mo1 43.2(9) . . . . ?
O31 P1A O7 Mo1 -175.2(5) . . . . ?
O24 P1A O7 Mo1 -61.5(6) . . . . ?
O1 P1A O7 Mo1 68.8(8) . . . . ?
O19 P2 O9 Mo2 111.3(4) . . . . ?
O25 P2 O9 Mo2 -13.9(5) . . . . ?
O12 P2 O9 Mo2 -130.0(4) . . . . ?
O19 P2 O9 Mo5 -98.4(4) . . . . ?
O25 P2 O9 Mo5 136.3(4) . . . . ?
O12 P2 O9 Mo5 20.2(5) . . . . ?
O28 P3 O11 Mo3 -28.0(7) . . . . ?
O21 P3 O11 Mo3 -146.8(6) 5_576 . . . ?
O27 P3 O11 Mo3 94.1(6) . . . . ?
O19 P2 O12 Mo6 101.3(4) . . . . ?
O25 P2 O12 Mo6 -133.3(4) . . . . ?
O9 P2 O12 Mo6 -18.3(5) . . . . ?
O19 P2 O12 Mo1 -114.7(4) . . . . ?
O25 P2 O12 Mo1 10.7(5) . . . . ?
O9 P2 O12 Mo1 125.7(4) . . . . ?
O30 P4 O17 Mo2 78.7(7) . . . . ?
O34 P4 O17 Mo2 -157.4(6) 2 . . . ?
O23 P4 O17 Mo2 -41.6(7) . . . . ?
O25 P2 O19 Co3 -73.4(6) . . . 2 ?
O9 P2 O19 Co3 166.3(5) . . . 2 ?
O12 P2 O19 Co3 47.9(6) . . . 2 ?
O25 P2 O19 Co2 78.9(5) . . . . ?
O9 P2 O19 Co2 -41.4(6) . . . . ?
O12 P2 O19 Co2 -159.7(4) . . . . ?
O30 P4 O23 Mo5 -77.1(6) . . . . ?
O34 P4 O23 Mo5 161.6(5) 2 . . . ?
O17 P4 O23 Mo5 46.4(6) . . . . ?
O31 P1A O24 Mo6 -179.4(6) . . . . ?
O1 P1A O24 Mo6 -54.0(11) . . . . ?
O7 P1A O24 Mo6 67.4(7) . . . . ?
O7 P1B O24 Mo6 -33.9(10) . . . . ?
O2 P1B O24 Mo6 96.6(11) . . . . ?
O31 P1B O24 Mo6 -151.4(7) . . . . ?
O19 P2 O25 Mo3 112.1(4) . . . . ?
O9 P2 O25 Mo3 -125.5(4) . . . . ?
O12 P2 O25 Mo3 -9.4(5) . . . . ?
O19 P2 O25 Mo4 -113.4(4) . . . . ?
O9 P2 O25 Mo4 9.0(5) . . . . ?
O12 P2 O25 Mo4 125.1(4) . . . . ?
O28 P3 O27 Co4 -115.6(4) . . . . ?
O21 P3 O27 Co4 1.8(6) 5_576 . . . ?
O11 P3 O27 Co4 121.2(4) . . . . ?
O21 P3 O28 Mo4 148.9(5) 5_576 . . . ?
O11 P3 O28 Mo4 29.2(7) . . . . ?
O27 P3 O28 Mo4 -93.0(6) . . . . ?
O34 P4 O30 Co2 -110.3(9) 2 . . . ?
O17 P4 O30 Co2 10.4(10) . . . . ?
O23 P4 O30 Co2 131.5(8) . . . . ?
O34 P4 O30 Co3 112.3(5) 2 . . . ?
O17 P4 O30 Co3 -127.0(4) . . . . ?
O23 P4 O30 Co3 -5.9(5) . . . . ?
C3 N2 C1 N1 7.7(17) . . . . ?
C4 N2 C1 N1 -172.2(13) . . . . ?
C2 N1 C1 N2 -1.1(14) . . . . ?
Co4 N1 C1 N2 -179.6(9) . . . . ?
C1 N1 C2 C3 -6.2(15) . . . . ?
Co4 N1 C2 C3 172.2(11) . . . . ?
C1 N2 C3 C2 -11.4(19) . . . . ?
C4 N2 C3 C2 168.5(15) . . . . ?
N1 C2 C3 N2 12(2) . . . . ?
C3 N2 C4 C5 69(2) . . . . ?
C1 N2 C4 C5 -111.4(17) . . . . ?
N2 C4 C5 C5 175.4(17) . . . 5_586 ?
C8 N4 C6 C7 1.4(15) . . . . ?
C9 N4 C6 C7 167.5(10) . . . . ?
C8 N3 C7 C6 0.4(15) . . . . ?
N4 C6 C7 N3 -1.1(15) . . . . ?
C7 N3 C8 N4 0.5(14) . . . . ?
C6 N4 C8 N3 -1.2(14) . . . . ?
C9 N4 C8 N3 -160.8(14) . . . . ?
C8 N4 C9 C10 81(2) . . . . ?
C6 N4 C9 C10 -79.2(16) . . . . ?
N4 C9 C10 C11 168.7(15) . . . . ?
C9 C10 C11 C12 -170.8(17) . . . . ?
C13 N5 C12 C11 -131.1(17) . . . . ?
C15 N5 C12 C11 49.6(19) . . . . ?
C10 C11 C12 N5 -166.8(15) . . . . ?
C15 N5 C13 C14 -2.1(14) . . . . ?
C12 N5 C13 C14 178.6(13) . . . . ?
N5 C13 C14 N6 8.5(15) . . . . ?
C15 N6 C14 C13 -11.3(15) . . . . ?
C14 N6 C15 N5 9.2(14) . . . . ?
C13 N5 C15 N6 -4.7(15) . . . . ?
C12 N5 C15 N6 174.8(11) . . . . ?

_refine_diff_density_max         2.307
_refine_diff_density_min         -1.808
_refine_diff_density_rms         0.268



####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_jw-27
_database_code_depnum_ccdc_archive 'CCDC 2062085'
loop_
_audit_author_name
_audit_author_address
'Yan Xu'
;Nanjing Tech University
China
;
_audit_update_record             
;
2021-05-13 deposited with the CCDC.	2021-05-24 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2018/3
_shelx_SHELXL_version_number     2018/3
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C40 H76.50 K2 Mo12 N16 O66 P8 Zn4.75'
_chemical_formula_weight         3625.42

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_H-M_alt        'C 2/c'
_space_group_name_Hall           '-C 2yc'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   30.91(4)
_cell_length_b                   14.749(16)
_cell_length_c                   25.10(3)
_cell_angle_alpha                90
_cell_angle_beta                 124.63(3)
_cell_angle_gamma                90
_cell_volume                     9417(19)
_cell_formula_units_Z            4
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    8653
_cell_measurement_theta_min      4.881
_cell_measurement_theta_max      54.029

_exptl_crystal_description       diamond-shaped
_exptl_crystal_colour            red
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    2.557
_exptl_crystal_F_000             7044
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.160
_exptl_crystal_size_mid          0.130
_exptl_crystal_size_min          0.120
_exptl_absorpt_coefficient_mu    3.066
_shelx_estimated_absorpt_T_min   0.640
_shelx_estimated_absorpt_T_max   0.710
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.634
_exptl_absorpt_correction_T_max  0.705
_exptl_absorpt_process_details   '(SADABS; Sheldrick, 2003)'
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker Apex2 CCD'
_diffrn_measurement_method       'ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            22961
_diffrn_reflns_av_unetI/netI     0.0760
_diffrn_reflns_av_R_equivalents  0.0803
_diffrn_reflns_limit_h_min       -32
_diffrn_reflns_limit_h_max       37
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_limit_l_max       30
_diffrn_reflns_theta_min         1.596
_diffrn_reflns_theta_max         25.500
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.972
_diffrn_measured_fraction_theta_full 0.975
_diffrn_reflns_Laue_measured_fraction_max 0.972
_diffrn_reflns_Laue_measured_fraction_full 0.975
_diffrn_reflns_point_group_measured_fraction_max 0.972
_diffrn_reflns_point_group_measured_fraction_full 0.975
_reflns_number_total             8532
_reflns_number_gt                7196
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       'APEX2 (Bruker, 2005)'
_computing_cell_refinement       'SAINT (Bruker, 2005)'
_computing_data_reduction        SAINT
_computing_structure_solution    'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_molecular_graphics    SHELXTL
_computing_publication_material  SHELXTL
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0726P)²] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         8532
_refine_ls_number_parameters     692
_refine_ls_number_restraints     139
_refine_ls_R_factor_all          0.0548
_refine_ls_R_factor_gt           0.0443
_refine_ls_wR_factor_ref         0.1320
_refine_ls_wR_factor_gt          0.1242
_refine_ls_goodness_of_fit_ref   1.074
_refine_ls_restrained_S_all      1.103
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.17796(2) -0.96866(3) 0.48635(2) 0.01379(14) Uani 1 1 d . . . . .
Mo2 Mo 0.19091(2) -0.95651(3) 0.39281(2) 0.01394(14) Uani 1 1 d . . . . .
Mo3 Mo 0.13429(2) -0.61903(3) 0.48230(2) 0.01554(14) Uani 1 1 d . . . . .
Mo4 Mo 0.14562(2) -0.77500(3) 0.53624(2) 0.01527(14) Uani 1 1 d . . . . .
Mo5 Mo 0.14636(2) -0.60691(3) 0.35236(2) 0.01650(14) Uani 1 1 d . . . . .
Mo6 Mo 0.17285(2) -0.74804(3) 0.31497(2) 0.01411(14) Uani 1 1 d . . . . .
Zn1 Zn -0.04135(3) -1.02273(5) 0.40677(3) 0.01692(17) Uani 1 1 d . . . . .
Zn2 Zn 0.250000 -0.750000 0.500000 0.0218(3) Uani 1 2 d S . P . .
Zn3 Zn 0.000000 -0.92661(7) 0.250000 0.0200(2) Uani 1 2 d S T P . .
Zn4 Zn 0.000000 -0.36732(11) 0.250000 0.0374(4) Uani 0.75 2 d S T P . .
P1 P 0.07599(6) -0.96664(10) 0.49821(7) 0.0154(3) Uani 1 1 d . . . . .
P2 P 0.10068(6) -0.80058(10) 0.37541(7) 0.0128(3) Uani 1 1 d . . . . .
P3 P 0.03896(7) -0.53238(12) 0.34240(8) 0.0268(4) Uani 1 1 d . . . . .
P4 P 0.10484(6) -0.93083(10) 0.23475(7) 0.0151(3) Uani 1 1 d . . . . .
K1 K 0.03107(7) -0.75812(12) 0.20250(9) 0.0454(5) Uani 1 1 d . . . . .
O1 O -0.00459(19) -0.6087(4) 0.3109(2) 0.0424(14) Uani 1 1 d . . . . .
O2 O 0.0117(2) -0.4410(4) 0.3213(3) 0.0452(15) Uani 1 1 d . . . . .
O3 O 0.1703(2) -0.5211(3) 0.3316(3) 0.0367(13) Uani 1 1 d . . . . .
O4 O 0.11068(15) -0.6973(2) 0.38999(18) 0.0139(9) Uani 1 1 d . . . . .
O5 O 0.19209(15) -0.7087(3) 0.51929(19) 0.0163(9) Uani 1 1 d . . . . .
O6 O 0.19789(16) -0.8838(3) 0.56349(19) 0.0178(9) Uani 1 1 d . . . . .
O7 O 0.13072(17) -0.8386(3) 0.24011(19) 0.0208(10) Uani 1 1 d . . . . .
O8 O 0.22238(15) -0.8869(3) 0.47431(19) 0.0151(9) Uani 1 1 d . . . . .
O9 O 0.20642(15) -0.6912(3) 0.40124(18) 0.0162(9) Uani 1 1 d . . . . .
O10 O 0.08413(16) -0.6999(3) 0.48085(19) 0.0191(9) Uani 1 1 d . . . . .
O11 O 0.14477(17) -0.9868(3) 0.29586(19) 0.0236(10) Uani 1 1 d . . . . .
O12 O 0.17054(16) -0.5539(3) 0.4434(2) 0.0191(9) Uani 1 1 d . . . . .
O13 O 0.10671(16) -0.6826(3) 0.27480(19) 0.0202(9) Uani 1 1 d . . . . .
O14 O 0.06978(16) -0.5429(3) 0.4156(2) 0.0245(10) Uani 1 1 d . . . . .
O15 O 0.02363(16) -0.9591(3) 0.43089(19) 0.0213(10) Uani 1 1 d . . . . .
O16 O 0.07381(17) -0.5434(3) 0.3166(2) 0.0224(10) Uani 1 1 d . . . . .
O17 O 0.20575(18) -0.7000(3) 0.2866(2) 0.0255(10) Uani 1 1 d . . . . .
O18 O 0.04402(15) -0.8189(3) 0.32248(19) 0.0176(9) Uani 1 1 d . . . . .
O19 O 0.16910(18) -0.7399(3) 0.6121(2) 0.0253(11) Uani 1 1 d . . . . .
O20 O 0.13736(16) -1.0145(3) 0.39853(19) 0.0173(9) Uani 1 1 d . . . . .
O21 O 0.22382(15) -0.8576(3) 0.36436(18) 0.0150(9) Uani 1 1 d . . . . .
O22 O 0.09471(17) -0.8713(3) 0.5276(2) 0.0203(10) Uani 1 1 d . . . . .
O23 O 0.13759(15) -0.8340(3) 0.35580(17) 0.0135(9) Uani 1 1 d . . . . .
O24 O 0.23638(17) -1.0385(3) 0.4137(2) 0.0227(10) Uani 1 1 d . . . . .
O25 O 0.11778(16) -1.0138(3) 0.49286(19) 0.0190(9) Uani 1 1 d . . . . .
O26 O 0.09782(17) -0.9810(3) 0.17784(19) 0.0244(10) Uani 1 1 d . . . . .
O27 O 0.15513(18) -0.5494(3) 0.5451(2) 0.0265(11) Uani 1 1 d . . . . .
O28 O 0.21981(17) -1.0524(3) 0.5313(2) 0.0224(10) Uani 1 1 d . . . . .
O29 O 0.12002(15) -0.8471(3) 0.44059(18) 0.0151(9) Uani 1 1 d . . . . .
O30 O 0.06706(17) -1.0221(3) 0.5428(2) 0.0236(10) Uani 1 1 d . . . . .
O32 O 0.05399(17) -0.9143(3) 0.2270(2) 0.0299(11) Uani 1 1 d . . . . .
O1W O 0.01244(19) -0.7755(3) 0.1000(2) 0.0405(14) Uani 1 1 d . . . . .
O2W O 0.03317(17) -1.0214(3) 0.3251(2) 0.0270(11) Uani 1 1 d . . . . .
N1 N -0.0259(2) -1.1553(4) 0.4062(3) 0.0294(14) Uani 1 1 d D . . . .
N2 N -0.0234(3) -1.3041(4) 0.4129(4) 0.0439(18) Uani 1 1 d . . . . .
N3 N -0.1327(3) -1.6719(4) 0.3894(4) 0.0481(19) Uani 1 1 d . . . . .
N4 N -0.1189(3) -1.8105(4) 0.4189(4) 0.052(2) Uani 1 1 d . . . . .
H4C H -0.109363 -1.866355 0.423200 0.063 Uiso 1 1 calc R U . . .
N5 N 0.0654(4) -0.2980(5) 0.2912(5) 0.082(3) Uani 1 1 d D . . . .
N6 N 0.1492(4) -0.2642(6) 0.3562(6) 0.108(4) Uani 1 1 d . U . . .
C1 C 0.0158(5) -1.2785(6) 0.4059(6) 0.085(4) Uani 1 1 d D U . . .
H1A H 0.039344 -1.316290 0.404744 0.101 Uiso 1 1 calc R U . . .
C2 C 0.0131(4) -1.1866(6) 0.4011(6) 0.085(4) Uani 1 1 d D U . . .
H2A H 0.034640 -1.150347 0.395104 0.102 Uiso 1 1 calc R U . . .
C3 C -0.0404(3) -1.2276(5) 0.4222(5) 0.049(2) Uani 1 1 d D U . . .
H3A H -0.060794 -1.225438 0.438570 0.059 Uiso 1 1 calc R U . . .
C4 C -0.0304(4) -1.3984(5) 0.4269(5) 0.052(2) Uani 1 1 d . . . . .
H4A H -0.001242 -1.434326 0.434225 0.062 Uiso 1 1 calc R U . . .
H4B H -0.028345 -1.398310 0.466974 0.062 Uiso 1 1 calc R U . . .
C5 C -0.0788(4) -1.4431(5) 0.3778(5) 0.060(3) Uani 1 1 d . . . . .
H5A H -0.079896 -1.449733 0.338617 0.072 Uiso 1 1 calc R U . . .
H5B H -0.108539 -1.406252 0.367754 0.072 Uiso 1 1 calc R U . . .
C6 C -0.0827(4) -1.5363(5) 0.4012(5) 0.065(3) Uani 1 1 d . . . . .
H6A H -0.055350 -1.574712 0.405604 0.078 Uiso 1 1 calc R U . . .
H6B H -0.075623 -1.529559 0.443932 0.078 Uiso 1 1 calc R U . . .
C7 C -0.1346(4) -1.5835(5) 0.3583(5) 0.057(3) Uani 1 1 d . . . . .
H7A H -0.162701 -1.545855 0.352588 0.068 Uiso 1 1 calc R U . . .
H7B H -0.141455 -1.594637 0.316060 0.068 Uiso 1 1 calc R U . . .
C8 C -0.1404(6) -1.7689(8) 0.4489(6) 0.093(4) Uani 1 1 d . U . . .
H8A H -0.147212 -1.795701 0.476903 0.112 Uiso 1 1 calc R U . . .
C9 C -0.1493(5) -1.6815(7) 0.4287(6) 0.086(4) Uani 1 1 d . U . . .
H9A H -0.163939 -1.636630 0.439798 0.103 Uiso 1 1 calc R U . . .
C10 C -0.1157(3) -1.7511(5) 0.3838(4) 0.043(2) Uani 1 1 d . U . . .
H10A H -0.103250 -1.762141 0.358269 0.051 Uiso 1 1 calc R U . . .
C11 C 0.2176(6) -0.2570(11) 0.4726(6) 0.129(6) Uani 1 1 d D U . . .
H11A H 0.205735 -0.309355 0.484347 0.155 Uiso 1 1 calc R U . . .
H11B H 0.199069 -0.204198 0.473037 0.155 Uiso 1 1 calc R U . . .
C12 C 0.2046(6) -0.2700(10) 0.4058(7) 0.131(6) Uani 1 1 d D U . . .
H12A H 0.222845 -0.224258 0.397757 0.158 Uiso 1 1 calc R U . . .
H12B H 0.217379 -0.328887 0.403333 0.158 Uiso 1 1 calc R U . . .
C13 C 0.1251(5) -0.1907(9) 0.3166(7) 0.124(5) Uani 1 1 d D U . . .
H13A H 0.140819 -0.137192 0.316292 0.148 Uiso 1 1 calc R U . . .
C14 C 0.0732(5) -0.2125(6) 0.2778(6) 0.108(5) Uani 1 1 d D U . . .
H14A H 0.046824 -0.174518 0.246709 0.129 Uiso 1 1 calc R U . . .
C15 C 0.1134(5) -0.3303(9) 0.3420(7) 0.095(4) Uani 1 1 d . U . . .
H15A H 0.120024 -0.386139 0.362457 0.113 Uiso 1 1 calc R U . . .
C16 C -0.2403(4) -1.3908(7) 0.2702(6) 0.078(3) Uani 1 1 d D U . . .
H16A H -0.225299 -1.347514 0.302932 0.093 Uiso 1 1 calc R U . . .
C17 C -0.2719(4) -1.4602(7) 0.2634(6) 0.081(4) Uani 1 1 d D U . . .
H17A H -0.283463 -1.471869 0.289794 0.097 Uiso 1 1 calc R U . . .
N7 N -0.2346(4) -1.3956(7) 0.2223(5) 0.100(4) Uani 1 1 d D U . . .
C18 C -0.2613(5) -1.4681(8) 0.1838(6) 0.109(5) Uani 1 1 d D U . . .
H18A H -0.263709 -1.485626 0.146632 0.130 Uiso 1 1 calc R U . . .
N8 N -0.2835(5) -1.5095(9) 0.2111(6) 0.146(5) Uani 1 1 d D U . . .
C19 C -0.2018(11) -1.3236(17) 0.2192(16) 0.130(11) Uani 0.5 1 d D U P . .
H19A H -0.173197 -1.356292 0.222507 0.156 Uiso 0.5 1 calc R U P . .
H19B H -0.223453 -1.300985 0.175172 0.156 Uiso 0.5 1 calc R U P . .
C22 C -0.1908(11) -1.1082(15) 0.2859(11) 0.109(9) Uani 0.5 1 d D U P . .
H22A H -0.158441 -1.093307 0.289984 0.131 Uiso 0.5 1 calc R U P . .
H22B H -0.180686 -1.141524 0.324655 0.131 Uiso 0.5 1 calc R U P . .
C21 C -0.2198(8) -1.1738(13) 0.2306(10) 0.079(7) Uani 0.5 1 d D U P . .
H21A H -0.252025 -1.195322 0.224468 0.094 Uiso 0.5 1 calc R U P . .
H21B H -0.227399 -1.148664 0.190440 0.094 Uiso 0.5 1 calc R U P . .
C20 C -0.1782(9) -1.2457(15) 0.2577(12) 0.093(8) Uani 0.5 1 d D U P . .
H20A H -0.149012 -1.225995 0.256080 0.111 Uiso 0.5 1 calc R U P . .
H20B H -0.165061 -1.258401 0.302397 0.111 Uiso 0.5 1 calc R U P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O28 1.677(4) . ?
Mo1 O20 1.936(4) . ?
Mo1 O8 1.975(4) . ?
Mo1 O25 2.068(5) . ?
Mo1 O6 2.084(4) . ?
Mo1 O29 2.325(4) . ?
Mo1 Mo2 2.603(3) . ?
Mo2 O24 1.696(4) . ?
Mo2 O20 1.940(5) . ?
Mo2 O8 1.980(4) . ?
Mo2 O11 2.052(5) . ?
Mo2 O21 2.121(4) . ?
Mo2 O23 2.260(4) . ?
Mo3 O27 1.674(4) . ?
Mo3 O10 1.940(4) . ?
Mo3 O5 1.979(4) . ?
Mo3 O14 2.060(4) . ?
Mo3 O12 2.092(5) . ?
Mo3 O4 2.305(4) . ?
Mo3 Mo4 2.590(2) . ?
Mo4 O19 1.688(5) . ?
Mo4 O10 1.942(4) . ?
Mo4 O5 1.974(4) . ?
Mo4 O22 2.038(5) . ?
Mo4 O6 2.097(4) . ?
Mo4 O29 2.315(5) . ?
Mo5 O3 1.691(5) . ?
Mo5 O13 1.956(4) . ?
Mo5 O9 1.977(4) . ?
Mo5 O16 2.103(5) . ?
Mo5 O12 2.110(5) . ?
Mo5 O4 2.252(4) . ?
Mo5 Mo6 2.599(2) . ?
Mo5 K1 4.073(4) . ?
Mo6 O17 1.693(5) . ?
Mo6 O13 1.945(5) . ?
Mo6 O9 1.979(4) . ?
Mo6 O7 2.056(4) . ?
Mo6 O21 2.100(4) . ?
Mo6 O23 2.261(4) . ?
Mo6 K1 3.625(5) . ?
Zn1 O26 1.930(4) 2 ?
Zn1 O30 1.954(5) 5_536 ?
Zn1 O15 1.974(5) . ?
Zn1 N1 2.015(6) . ?
Zn2 O8 2.144(4) . ?
Zn2 O8 2.145(4) 7_536 ?
Zn2 O5 2.190(5) 7_536 ?
Zn2 O5 2.190(5) . ?
Zn2 O9 2.218(5) . ?
Zn2 O9 2.218(5) 7_536 ?
Zn3 O32 2.060(5) . ?
Zn3 O32 2.060(5) 2 ?
Zn3 O2W 2.089(5) 2 ?
Zn3 O2W 2.089(5) . ?
Zn3 O18 2.207(4) 2 ?
Zn3 O18 2.207(4) . ?
Zn3 K1 3.134(3) 2 ?
Zn3 K1 3.134(3) . ?
Zn4 O2 1.943(6) . ?
Zn4 O2 1.944(6) 2 ?
Zn4 N5 1.955(9) 2 ?
Zn4 N5 1.955(9) . ?
P1 O30 1.532(5) . ?
P1 O25 1.539(5) . ?
P1 O22 1.539(4) . ?
P1 O15 1.542(4) . ?
P2 O18 1.504(4) . ?
P2 O29 1.547(4) . ?
P2 O23 1.557(4) . ?
P2 O4 1.555(4) . ?
P2 K1 3.428(5) 2 ?
P2 K1 3.640(5) . ?
P3 O2 1.516(5) . ?
P3 O14 1.522(5) . ?
P3 O16 1.549(5) . ?
P3 O1 1.580(5) . ?
P3 K1 3.777(4) 2 ?
P4 O32 1.491(5) . ?
P4 O26 1.511(4) . ?
P4 O7 1.545(5) . ?
P4 O11 1.551(4) . ?
P4 K1 3.201(4) . ?
K1 O18 2.220(5) 2 ?
K1 O13 2.276(5) . ?
K1 O1 2.308(6) 2 ?
K1 O1W 2.310(7) . ?
K1 O32 2.385(6) . ?
K1 O7 2.912(6) . ?
K1 O18 2.943(6) . ?
N1 C3 1.305(9) . ?
N1 C2 1.362(3) . ?
N2 C3 1.318(10) . ?
N2 C1 1.373(13) . ?
N2 C4 1.480(9) . ?
N3 C10 1.321(10) . ?
N3 C9 1.352(13) . ?
N3 C7 1.503(10) . ?
N4 C10 1.286(10) . ?
N4 C8 1.398(14) . ?
N4 H4C 0.8600 . ?
N5 C14 1.360(2) . ?
N5 C15 1.381(15) . ?
N6 C15 1.361(14) . ?
N6 C13 1.370(16) . ?
N6 C12 1.438(16) . ?
C1 C2 1.360(3) . ?
C1 H1A 0.9300 . ?
C2 H2A 0.9300 . ?
C3 H3A 0.9300 . ?
C4 C5 1.447(13) . ?
C4 H4A 0.9700 . ?
C4 H4B 0.9700 . ?
C5 C6 1.526(11) . ?
C5 H5A 0.9700 . ?
C5 H5B 0.9700 . ?
C6 C7 1.504(13) . ?
C6 H6A 0.9700 . ?
C6 H6B 0.9700 . ?
C7 H7A 0.9700 . ?
C7 H7B 0.9700 . ?
C8 C9 1.354(15) . ?
C8 H8A 0.9300 . ?
C9 H9A 0.9300 . ?
C10 H10A 0.9300 . ?
C11 C12 1.500(3) . ?
C11 C11 1.68(3) 7_546 ?
C11 H11A 0.9700 . ?
C11 H11B 0.9700 . ?
C12 H12A 0.9700 . ?
C12 H12B 0.9700 . ?
C13 C14 1.360(3) . ?
C13 H13A 0.9300 . ?
C14 H14A 0.9300 . ?
C15 H15A 0.9300 . ?
C16 N7 1.310(14) . ?
C16 C17 1.358(2) . ?
C16 H16A 0.9300 . ?
C17 N8 1.359(2) . ?
C17 H17A 0.9300 . ?
N7 C18 1.360(2) . ?
N7 C19 1.500(2) . ?
C18 N8 1.360(2) . ?
C18 H18A 0.9300 . ?
N8 C22 1.68(3) 4_445 ?
C19 C20 1.41(3) . ?
C19 H19A 0.9700 . ?
C19 H19B 0.9700 . ?
C22 C21 1.500(2) . ?
C22 H22A 0.9700 . ?
C22 H22B 0.9700 . ?
C21 C20 1.500(2) . ?
C21 H21A 0.9700 . ?
C21 H21B 0.9700 . ?
C20 H20A 0.9700 . ?
C20 H20B 0.9700 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O28 Mo1 O20 105.1(2) . . ?
O28 Mo1 O8 102.4(2) . . ?
O20 Mo1 O8 95.52(18) . . ?
O28 Mo1 O25 95.4(2) . . ?
O20 Mo1 O25 86.98(18) . . ?
O8 Mo1 O25 160.64(16) . . ?
O28 Mo1 O6 96.3(2) . . ?
O20 Mo1 O6 157.86(17) . . ?
O8 Mo1 O6 84.91(17) . . ?
O25 Mo1 O6 85.66(17) . . ?
O28 Mo1 O29 169.63(18) . . ?
O20 Mo1 O29 83.58(16) . . ?
O8 Mo1 O29 82.01(18) . . ?
O25 Mo1 O29 79.20(17) . . ?
O6 Mo1 O29 74.54(16) . . ?
O28 Mo1 Mo2 101.63(17) . . ?
O20 Mo1 Mo2 47.88(15) . . ?
O8 Mo1 Mo2 48.94(12) . . ?
O25 Mo1 Mo2 134.43(11) . . ?
O6 Mo1 Mo2 132.93(13) . . ?
O29 Mo1 Mo2 88.36(12) . . ?
O24 Mo2 O20 104.8(2) . . ?
O24 Mo2 O8 102.49(19) . . ?
O20 Mo2 O8 95.21(18) . . ?
O24 Mo2 O11 96.1(2) . . ?
O20 Mo2 O11 86.82(19) . . ?
O8 Mo2 O11 160.06(17) . . ?
O24 Mo2 O21 97.0(2) . . ?
O20 Mo2 O21 157.08(16) . . ?
O8 Mo2 O21 86.77(17) . . ?
O11 Mo2 O21 83.88(18) . . ?
O24 Mo2 O23 168.61(18) . . ?
O20 Mo2 O23 85.96(18) . . ?
O8 Mo2 O23 79.96(16) . . ?
O11 Mo2 O23 80.41(16) . . ?
O21 Mo2 O23 71.87(17) . . ?
O24 Mo2 Mo1 101.40(16) . . ?
O20 Mo2 Mo1 47.75(12) . . ?
O8 Mo2 Mo1 48.76(13) . . ?
O11 Mo2 Mo1 134.05(16) . . ?
O21 Mo2 Mo1 134.45(11) . . ?
O23 Mo2 Mo1 88.61(11) . . ?
O27 Mo3 O10 105.7(2) . . ?
O27 Mo3 O5 101.9(2) . . ?
O10 Mo3 O5 95.57(19) . . ?
O27 Mo3 O14 96.2(2) . . ?
O10 Mo3 O14 85.7(2) . . ?
O5 Mo3 O14 160.73(17) . . ?
O27 Mo3 O12 97.9(2) . . ?
O10 Mo3 O12 155.24(17) . . ?
O5 Mo3 O12 86.88(19) . . ?
O14 Mo3 O12 84.2(2) . . ?
O27 Mo3 O4 170.72(19) . . ?
O10 Mo3 O4 83.12(17) . . ?
O5 Mo3 O4 79.78(16) . . ?
O14 Mo3 O4 81.29(17) . . ?
O12 Mo3 O4 73.05(16) . . ?
O27 Mo3 Mo4 100.78(18) . . ?
O10 Mo3 Mo4 48.18(13) . . ?
O5 Mo3 Mo4 48.97(13) . . ?
O14 Mo3 Mo4 133.60(14) . . ?
O12 Mo3 Mo4 134.65(12) . . ?
O4 Mo3 Mo4 87.25(12) . . ?
O19 Mo4 O10 104.5(2) . . ?
O19 Mo4 O5 101.1(2) . . ?
O10 Mo4 O5 95.68(19) . . ?
O19 Mo4 O22 98.36(19) . . ?
O10 Mo4 O22 86.5(2) . . ?
O5 Mo4 O22 159.20(17) . . ?
O19 Mo4 O6 96.3(2) . . ?
O10 Mo4 O6 158.37(17) . . ?
O5 Mo4 O6 85.93(19) . . ?
O22 Mo4 O6 84.64(19) . . ?
O19 Mo4 O29 170.04(18) . . ?
O10 Mo4 O29 84.31(17) . . ?
O5 Mo4 O29 82.28(16) . . ?
O22 Mo4 O29 77.35(16) . . ?
O6 Mo4 O29 74.51(15) . . ?
O19 Mo4 Mo3 99.26(17) . . ?
O10 Mo4 Mo3 48.10(13) . . ?
O5 Mo4 Mo3 49.15(12) . . ?
O22 Mo4 Mo3 134.15(13) . . ?
O6 Mo4 Mo3 134.44(13) . . ?
O29 Mo4 Mo3 90.03(12) . . ?
O3 Mo5 O13 104.9(2) . . ?
O3 Mo5 O9 103.9(2) . . ?
O13 Mo5 O9 95.47(18) . . ?
O3 Mo5 O16 94.7(2) . . ?
O13 Mo5 O16 85.20(18) . . ?
O9 Mo5 O16 160.42(17) . . ?
O3 Mo5 O12 96.2(2) . . ?
O13 Mo5 O12 157.72(17) . . ?
O9 Mo5 O12 86.03(17) . . ?
O16 Mo5 O12 86.14(17) . . ?
O3 Mo5 O4 167.7(2) . . ?
O13 Mo5 O4 84.27(18) . . ?
O9 Mo5 O4 83.01(18) . . ?
O16 Mo5 O4 77.58(17) . . ?
O12 Mo5 O4 73.83(16) . . ?
O3 Mo5 Mo6 101.86(19) . . ?
O13 Mo5 Mo6 48.05(13) . . ?
O9 Mo5 Mo6 48.95(13) . . ?
O16 Mo5 Mo6 132.89(12) . . ?
O12 Mo5 Mo6 134.21(12) . . ?
O4 Mo5 Mo6 90.40(12) . . ?
O3 Mo5 K1 115.6(2) . . ?
O13 Mo5 K1 17.02(13) . . ?
O9 Mo5 K1 104.44(14) . . ?
O16 Mo5 K1 71.85(14) . . ?
O12 Mo5 K1 142.06(13) . . ?
O4 Mo5 K1 71.52(13) . . ?
Mo6 Mo5 K1 61.18(8) . . ?
O17 Mo6 O13 106.3(2) . . ?
O17 Mo6 O9 102.5(2) . . ?
O13 Mo6 O9 95.73(17) . . ?
O17 Mo6 O7 96.1(2) . . ?
O13 Mo6 O7 85.14(18) . . ?
O9 Mo6 O7 160.27(16) . . ?
O17 Mo6 O21 98.1(2) . . ?
O13 Mo6 O21 154.50(17) . . ?
O9 Mo6 O21 85.95(17) . . ?
O7 Mo6 O21 85.01(17) . . ?
O17 Mo6 O23 169.90(19) . . ?
O13 Mo6 O23 82.98(18) . . ?
O9 Mo6 O23 80.19(17) . . ?
O7 Mo6 O23 80.35(17) . . ?
O21 Mo6 O23 72.21(17) . . ?
O17 Mo6 Mo5 101.81(17) . . ?
O13 Mo6 Mo5 48.40(13) . . ?
O9 Mo6 Mo5 48.88(12) . . ?
O7 Mo6 Mo5 133.16(14) . . ?
O21 Mo6 Mo5 133.44(13) . . ?
O23 Mo6 Mo5 87.33(12) . . ?
O17 Mo6 K1 116.03(18) . . ?
O13 Mo6 K1 33.62(13) . . ?
O9 Mo6 K1 121.31(12) . . ?
O7 Mo6 K1 53.42(13) . . ?
O21 Mo6 K1 126.71(12) . . ?
O23 Mo6 K1 69.46(13) . . ?
Mo5 Mo6 K1 79.90(7) . . ?
O26 Zn1 O30 99.1(2) 2 5_536 ?
O26 Zn1 O15 108.19(19) 2 . ?
O30 Zn1 O15 111.0(2) 5_536 . ?
O26 Zn1 N1 111.8(2) 2 . ?
O30 Zn1 N1 121.2(2) 5_536 . ?
O15 Zn1 N1 105.0(2) . . ?
O8 Zn2 O8 180.0 . 7_536 ?
O8 Zn2 O5 84.68(16) . 7_536 ?
O8 Zn2 O5 95.32(16) 7_536 7_536 ?
O8 Zn2 O5 95.32(16) . . ?
O8 Zn2 O5 84.68(16) 7_536 . ?
O5 Zn2 O5 180.00(8) 7_536 . ?
O8 Zn2 O9 98.48(15) . . ?
O8 Zn2 O9 81.53(15) 7_536 . ?
O5 Zn2 O9 85.15(17) 7_536 . ?
O5 Zn2 O9 94.86(17) . . ?
O8 Zn2 O9 81.53(15) . 7_536 ?
O8 Zn2 O9 98.47(15) 7_536 7_536 ?
O5 Zn2 O9 94.85(17) 7_536 7_536 ?
O5 Zn2 O9 85.14(17) . 7_536 ?
O9 Zn2 O9 180.0 . 7_536 ?
O32 Zn3 O32 169.9(3) . 2 ?
O32 Zn3 O2W 82.3(2) . 2 ?
O32 Zn3 O2W 104.6(2) 2 2 ?
O32 Zn3 O2W 104.6(2) . . ?
O32 Zn3 O2W 82.3(2) 2 . ?
O2W Zn3 O2W 96.0(3) 2 . ?
O32 Zn3 O18 85.62(19) . 2 ?
O32 Zn3 O18 87.09(19) 2 2 ?
O2W Zn3 O18 88.93(18) 2 2 ?
O2W Zn3 O18 169.16(17) . 2 ?
O32 Zn3 O18 87.08(19) . . ?
O32 Zn3 O18 85.62(19) 2 . ?
O2W Zn3 O18 169.16(17) 2 . ?
O2W Zn3 O18 88.93(18) . . ?
O18 Zn3 O18 87.9(2) 2 . ?
O32 Zn3 K1 120.57(16) . 2 ?
O32 Zn3 K1 49.56(15) 2 2 ?
O2W Zn3 K1 140.79(13) 2 2 ?
O2W Zn3 K1 106.66(16) . 2 ?
O18 Zn3 K1 64.16(14) 2 2 ?
O18 Zn3 K1 45.11(13) . 2 ?
O32 Zn3 K1 49.56(15) . . ?
O32 Zn3 K1 120.57(16) 2 . ?
O2W Zn3 K1 106.66(16) 2 . ?
O2W Zn3 K1 140.79(13) . . ?
O18 Zn3 K1 45.11(13) 2 . ?
O18 Zn3 K1 64.16(14) . . ?
K1 Zn3 K1 75.08(11) 2 . ?
O2 Zn4 O2 112.0(3) . 2 ?
O2 Zn4 N5 112.0(3) . 2 ?
O2 Zn4 N5 102.1(3) 2 2 ?
O2 Zn4 N5 102.1(3) . . ?
O2 Zn4 N5 112.0(3) 2 . ?
N5 Zn4 N5 116.9(5) 2 . ?
O30 P1 O25 109.3(2) . . ?
O30 P1 O22 108.2(3) . . ?
O25 P1 O22 110.4(2) . . ?
O30 P1 O15 109.0(3) . . ?
O25 P1 O15 110.3(3) . . ?
O22 P1 O15 109.5(2) . . ?
O18 P2 O29 114.3(2) . . ?
O18 P2 O23 111.0(3) . . ?
O29 P2 O23 106.4(2) . . ?
O18 P2 O4 111.1(2) . . ?
O29 P2 O4 106.2(2) . . ?
O23 P2 O4 107.5(2) . . ?
O18 P2 K1 28.24(16) . 2 ?
O29 P2 K1 107.71(17) . 2 ?
O23 P2 K1 136.37(17) . 2 ?
O4 P2 K1 88.18(16) . 2 ?
O18 P2 K1 51.30(17) . . ?
O29 P2 K1 161.60(16) . . ?
O23 P2 K1 73.76(16) . . ?
O4 P2 K1 90.91(15) . . ?
K1 P2 K1 65.33(7) 2 . ?
O2 P3 O14 110.8(3) . . ?
O2 P3 O16 109.1(3) . . ?
O14 P3 O16 112.8(3) . . ?
O2 P3 O1 108.2(3) . . ?
O14 P3 O1 107.6(3) . . ?
O16 P3 O1 108.2(3) . . ?
O2 P3 K1 124.7(3) . 2 ?
O14 P3 K1 97.44(19) . 2 ?
O16 P3 K1 101.50(19) . 2 ?
O1 P3 K1 16.6(2) . 2 ?
O32 P4 O26 112.5(3) . . ?
O32 P4 O7 108.8(3) . . ?
O26 P4 O7 107.6(3) . . ?
O32 P4 O11 113.8(3) . . ?
O26 P4 O11 106.3(3) . . ?
O7 P4 O11 107.5(2) . . ?
O32 P4 K1 44.7(2) . . ?
O26 P4 K1 116.84(19) . . ?
O7 P4 K1 65.2(2) . . ?
O11 P4 K1 136.52(19) . . ?
O18 K1 O13 149.11(19) 2 . ?
O18 K1 O1 96.72(19) 2 2 ?
O13 K1 O1 76.55(18) . 2 ?
O18 K1 O1W 94.70(18) 2 . ?
O13 K1 O1W 115.82(19) . . ?
O1 K1 O1W 95.8(2) 2 . ?
O18 K1 O32 78.03(17) 2 . ?
O13 K1 O32 104.29(17) . . ?
O1 K1 O32 171.2(2) 2 . ?
O1W K1 O32 91.70(18) . . ?
O18 K1 O7 132.11(17) 2 . ?
O13 K1 O7 61.49(16) . . ?
O1 K1 O7 131.17(17) 2 . ?
O1W K1 O7 82.18(16) . . ?
O32 K1 O7 54.46(14) . . ?
O18 K1 O18 71.24(16) 2 . ?
O13 K1 O18 81.51(16) . . ?
O1 K1 O18 105.69(18) 2 . ?
O1W K1 O18 155.36(17) . . ?
O32 K1 O18 66.06(14) . . ?
O7 K1 O18 92.32(13) . . ?
O18 K1 Zn3 44.77(10) 2 . ?
O13 K1 Zn3 118.87(14) . . ?
O1 K1 Zn3 130.73(17) 2 . ?
O1W K1 Zn3 113.54(15) . . ?
O32 K1 Zn3 41.10(13) . . ?
O7 K1 Zn3 92.87(12) . . ?
O18 K1 Zn3 42.45(8) . . ?
O18 K1 P4 103.32(15) 2 . ?
O13 K1 P4 85.78(15) . . ?
O1 K1 P4 159.95(16) 2 . ?
O1W K1 P4 83.34(14) . . ?
O32 K1 P4 26.09(12) . . ?
O7 K1 P4 28.79(9) . . ?
O18 K1 P4 80.55(10) . . ?
Zn3 K1 P4 66.49(9) . . ?
O18 K1 P2 18.69(11) 2 2 ?
O13 K1 P2 153.32(14) . 2 ?
O1 K1 P2 83.30(15) 2 2 ?
O1W K1 P2 83.16(14) . 2 ?
O32 K1 P2 93.05(13) . 2 ?
O7 K1 P2 143.65(12) . 2 ?
O18 K1 P2 87.41(11) . 2 ?
Zn3 K1 P2 63.29(6) . 2 ?
P4 K1 P2 116.33(9) . 2 ?
O18 K1 Mo6 147.54(13) 2 . ?
O13 K1 Mo6 28.25(11) . . ?
O1 K1 Mo6 104.24(14) 2 . ?
O1W K1 Mo6 107.33(16) . . ?
O32 K1 Mo6 77.77(12) . . ?
O7 K1 Mo6 34.54(10) . . ?
O18 K1 Mo6 79.30(11) . . ?
Zn3 K1 Mo6 103.44(8) . . ?
P4 K1 Mo6 57.54(7) . . ?
P2 K1 Mo6 166.05(7) 2 . ?
O18 K1 P2 94.70(13) 2 . ?
O13 K1 P2 59.33(12) . . ?
O1 K1 P2 104.96(15) 2 . ?
O1W K1 P2 156.01(15) . . ?
O32 K1 P2 68.80(12) . . ?
O7 K1 P2 75.15(10) . . ?
O18 K1 P2 23.50(9) . . ?
Zn3 K1 P2 60.73(6) . . ?
P4 K1 P2 73.03(6) . . ?
P2 K1 P2 110.76(7) 2 . ?
Mo6 K1 P2 56.25(5) . . ?
P3 O1 K1 152.1(3) . 2 ?
P3 O2 Zn4 126.6(3) . . ?
P2 O4 Mo5 124.1(2) . . ?
P2 O4 Mo3 129.3(2) . . ?
Mo5 O4 Mo3 100.03(16) . . ?
Mo4 O5 Mo3 81.87(18) . . ?
Mo4 O5 Zn2 134.1(2) . . ?
Mo3 O5 Zn2 135.7(2) . . ?
Mo1 O6 Mo4 112.99(18) . . ?
P4 O7 Mo6 132.8(3) . . ?
P4 O7 K1 86.0(2) . . ?
Mo6 O7 K1 92.04(17) . . ?
Mo1 O8 Mo2 82.29(16) . . ?
Mo1 O8 Zn2 136.2(2) . . ?
Mo2 O8 Zn2 132.6(2) . . ?
Mo5 O9 Mo6 82.17(16) . . ?
Mo5 O9 Zn2 134.4(2) . . ?
Mo6 O9 Zn2 131.7(2) . . ?
Mo3 O10 Mo4 83.72(19) . . ?
P4 O11 Mo2 133.1(3) . . ?
Mo3 O12 Mo5 112.43(19) . . ?
Mo6 O13 Mo5 83.56(17) . . ?
Mo6 O13 K1 118.1(2) . . ?
Mo5 O13 K1 148.4(2) . . ?
P3 O14 Mo3 133.6(3) . . ?
P1 O15 Zn1 123.6(3) . . ?
P3 O16 Mo5 134.0(3) . . ?
P2 O18 Zn3 136.1(2) . . ?
P2 O18 K1 133.1(3) . 2 ?
Zn3 O18 K1 90.11(16) . 2 ?
P2 O18 K1 105.2(2) . . ?
Zn3 O18 K1 73.39(14) . . ?
K1 O18 K1 94.35(15) 2 . ?
Mo1 O20 Mo2 84.36(17) . . ?
Mo6 O21 Mo2 112.7(2) . . ?
P1 O22 Mo4 138.2(3) . . ?
P2 O23 Mo2 128.1(2) . . ?
P2 O23 Mo6 126.5(2) . . ?
Mo2 O23 Mo6 101.99(18) . . ?
P1 O25 Mo1 134.3(3) . . ?
P4 O26 Zn1 138.7(3) . 2 ?
P2 O29 Mo4 126.3(2) . . ?
P2 O29 Mo1 126.2(2) . . ?
Mo4 O29 Mo1 97.38(15) . . ?
P1 O30 Zn1 127.0(3) . 5_536 ?
P4 O32 Zn3 155.7(3) . . ?
P4 O32 K1 109.2(3) . . ?
Zn3 O32 K1 89.34(19) . . ?
C3 N1 C2 103.2(6) . . ?
C3 N1 Zn1 131.8(5) . . ?
C2 N1 Zn1 123.7(5) . . ?
C3 N2 C1 104.8(7) . . ?
C3 N2 C4 129.5(7) . . ?
C1 N2 C4 123.2(7) . . ?
C10 N3 C9 108.9(8) . . ?
C10 N3 C7 127.7(8) . . ?
C9 N3 C7 123.4(8) . . ?
C10 N4 C8 108.3(8) . . ?
C10 N4 H4C 125.8 . . ?
C8 N4 H4C 125.8 . . ?
C14 N5 C15 107.4(10) . . ?
C14 N5 Zn4 129.0(8) . . ?
C15 N5 Zn4 123.6(8) . . ?
C15 N6 C13 110.5(11) . . ?
C15 N6 C12 125.1(12) . . ?
C13 N6 C12 124.4(11) . . ?
C2 C1 N2 105.8(9) . . ?
C2 C1 H1A 127.1 . . ?
N2 C1 H1A 127.1 . . ?
C1 C2 N1 110.0(8) . . ?
C1 C2 H2A 125.0 . . ?
N1 C2 H2A 125.0 . . ?
N1 C3 N2 113.9(7) . . ?
N1 C3 H3A 123.0 . . ?
N2 C3 H3A 123.0 . . ?
C5 C4 N2 116.5(8) . . ?
C5 C4 H4A 108.2 . . ?
N2 C4 H4A 108.2 . . ?
C5 C4 H4B 108.2 . . ?
N2 C4 H4B 108.2 . . ?
H4A C4 H4B 107.3 . . ?
C4 C5 C6 110.6(8) . . ?
C4 C5 H5A 109.5 . . ?
C6 C5 H5A 109.5 . . ?
C4 C5 H5B 109.5 . . ?
C6 C5 H5B 109.5 . . ?
H5A C5 H5B 108.1 . . ?
C7 C6 C5 115.3(8) . . ?
C7 C6 H6A 108.4 . . ?
C5 C6 H6A 108.4 . . ?
C7 C6 H6B 108.4 . . ?
C5 C6 H6B 108.4 . . ?
H6A C6 H6B 107.5 . . ?
N3 C7 C6 108.6(7) . . ?
N3 C7 H7A 110.0 . . ?
C6 C7 H7A 110.0 . . ?
N3 C7 H7B 110.0 . . ?
C6 C7 H7B 110.0 . . ?
H7A C7 H7B 108.3 . . ?
C9 C8 N4 105.9(10) . . ?
C9 C8 H8A 127.0 . . ?
N4 C8 H8A 127.0 . . ?
N3 C9 C8 107.0(10) . . ?
N3 C9 H9A 126.5 . . ?
C8 C9 H9A 126.5 . . ?
N4 C10 N3 109.9(8) . . ?
N4 C10 H10A 125.1 . . ?
N3 C10 H10A 125.1 . . ?
C12 C11 C11 111.6(15) . 7_546 ?
C12 C11 H11A 109.3 . . ?
C11 C11 H11A 109.3 7_546 . ?
C12 C11 H11B 109.3 . . ?
C11 C11 H11B 109.3 7_546 . ?
H11A C11 H11B 108.0 . . ?
N6 C12 C11 113.0(14) . . ?
N6 C12 H12A 109.0 . . ?
C11 C12 H12A 109.0 . . ?
N6 C12 H12B 109.0 . . ?
C11 C12 H12B 109.0 . . ?
H12A C12 H12B 107.8 . . ?
C14 C13 N6 105.5(11) . . ?
C14 C13 H13A 127.3 . . ?
N6 C13 H13A 127.3 . . ?
C13 C14 N5 110.2(11) . . ?
C13 C14 H14A 124.9 . . ?
N5 C14 H14A 124.9 . . ?
N6 C15 N5 106.4(11) . . ?
N6 C15 H15A 126.8 . . ?
N5 C15 H15A 126.8 . . ?
N7 C16 C17 107.8(9) . . ?
N7 C16 H16A 126.1 . . ?
C17 C16 H16A 126.1 . . ?
C16 C17 N8 107.5(10) . . ?
C16 C17 H17A 126.3 . . ?
N8 C17 H17A 126.3 . . ?
C16 N7 C18 110.6(10) . . ?
C16 N7 C19 117.1(15) . . ?
C18 N7 C19 132.3(17) . . ?
N8 C18 N7 105.7(11) . . ?
N8 C18 H18A 127.1 . . ?
N7 C18 H18A 127.1 . . ?
C17 N8 C18 108.3(11) . . ?
C17 N8 C22 107.0(12) . 4_445 ?
C18 N8 C22 143.1(13) . 4_445 ?
C20 C19 N7 130(3) . . ?
C20 C19 H19A 104.7 . . ?
N7 C19 H19A 104.7 . . ?
C20 C19 H19B 104.7 . . ?
N7 C19 H19B 104.7 . . ?
H19A C19 H19B 105.7 . . ?
C21 C22 N8 123.4(19) . 4_455 ?
C21 C22 H22A 106.5 . . ?
N8 C22 H22A 106.5 4_455 . ?
C21 C22 H22B 106.5 . . ?
N8 C22 H22B 106.5 4_455 . ?
H22A C22 H22B 106.5 . . ?
C20 C21 C22 97.4(18) . . ?
C20 C21 H21A 112.3 . . ?
C22 C21 H21A 112.3 . . ?
C20 C21 H21B 112.3 . . ?
C22 C21 H21B 112.3 . . ?
H21A C21 H21B 109.9 . . ?
C19 C20 C21 107(2) . . ?
C19 C20 H20A 110.4 . . ?
C21 C20 H20A 110.4 . . ?
C19 C20 H20B 110.4 . . ?
C21 C20 H20B 110.4 . . ?
H20A C20 H20B 108.6 . . ?

_refine_diff_density_max         1.267
_refine_diff_density_min         -1.412
_refine_diff_density_rms         0.225



